Functionalized Zeolitic Imidazolate Frameworks
Tuning the Responsive Phase Transition and Melting Behavior
Functionalized Zeolitic Imidazolate Frameworks
Tuning the Responsive Phase Transition and Melting Behavior
Faculty of Chemistry and Chemical Biology Technische Universität Dortmund
Dissertation Submitted by
This work was performed between September 2019 and February 2023 in the Inorganic Chemistry Department of the Faculty of Chemistry and Chemical Biology − Technische Universität Dortmund.
1st referee: Prof. Dr. Sebastian Henke 2nd referee: Prof. Dr. Guido Clever Date of submission: 15.02.2023 Date of examination: 20.03.2023
Life is a way to find yourself.
I hereby express my deepest gratitude to my supervisor Prof. Dr. Sebastian Henke
for accepting me as his student, giving me a chance to study the exciting MOFs and instructing me meticulously throughout my Ph.D. studying,
without him this dissertation cannot be accomplished.
I also thank Prof. Dr. Guido Clever for being the second referee of this dissertation.
I would first like to thank my colleagues, Louis Frentzel-Beyme, Roman Pallach, Pascal Kolodzeiski and Kai Terlinden, who performed the high energy X-ray characterization with me at Diamond Light Source (DLS) and Deutsches Elektronen-Synchrotron (DESY), and the beamline scientists at different synchrotrons for helping me with the crucial measurements supporting this work.
I would then like to thank my students Wenshu Wang (preliminary trials with the mechanochemical syntheses), Jonathan Pöttker (mechanochemically synthesizing cyano-functionalized samples) and Lorenzo Hiltmann (investigating the liquid-liquid transition of cyano-functionalized ZIF-4) for synthesizing the samples and performing the characterizations in this work.
I would like to sincerely thank my colleagues, who helped me to peer review this thesis: Chinmoy Das, Louis Frentzel-Beyme, Roman Pallach, Pascal Kolodzeiski, Kai Terlinden, Wenong Xue and Jan-Benedikt Weiß; who revised the abstract in Germen: Roman Pallach, Pascal Kolodzeiski and Jan-Benedikt Weiß.
I would like to thank my colleague Louis Frentzel-Beyme for helping me to settle down in Dortmund, instructing me with the syntheses at the beginning, and discussing scientific questions with me.
I would like to especially thank my colleague Kai Terlinden for organizing all kinds of events on the Mid-Autumn’s Day, Spring Festival and Dragon Boat’s Day for me and playing traditional music on those days, which drove my homesick away on those family reunion occasions.
Furthermore, I would like to also thank the colleagues from the neighboring groups (Clever group, Steffen group, etc.) or other departments who provided me many conveniences throughout my studying here at TU Dortmund.
The atmosphere in our group is like a big family, I thank all our family members:
Sebastian Henke, Athanasios Koutsianos, Chinmoy Das, Louis Frentzel-Beyme, Roman Pallach, Pascal Kolodzeiski, Kai Terlinden, Wenong Xue, Jan-Benedikt Weiß, Jannik Engel, ..., for your accompanies, having lunch with me, discussing different information with me, go to different events with me, traveling to different places with me and so on, which really adjusted my foreign life here.
Last but not least, I would like to thank my family, who always give me their selfless love through the screens due to the distance and the pandemic situation.
My parents are really uncomplainable, they will do anything they can to love me. My sister can always provide suitable suggestions for dealing with the academic issues. My brother always encourages me to stay calm and think more.
They are my strongest backup force.
Finally, I would also like to thank myself, for being so brave to stand alone abroad. Being in an opposite culture, so many things in my mind need to be turned upside down and set up again, in order to get adapted. The thinking atmosphere here thankfully helped me to reflect on myself more, where my interests are and what my advantage is. Anyhow, it’s an interesting piece of my life here, and I will keep going to find a better myself.
Metal-organic frameworks (MOFs) are showing various structure flexibility in response to external stimuli (e.g., pressures and temperatures). Their responsiveness can be manipulated by the substitution of the functional groups at the organic linker of the frameworks. Some MOFs are recently reported to be able to melt and form glasses, and their melting behavior is also related to functionalizing the linkers. Thus, the mechanisms of controlling responsiveness and melting behaviors of MOFs by linker functionalization (using benzo and cyano groups) have been studied in this work.
The high-pressure behavior of a series of Zeolitic Imidazolate Frameworks (ZIFs) of ZIF-62 (M(im)2-x(bim)x, M = Zn2+/Co2+, im– = imidazolate, bim– = benzimidazolate, 0.02 x 0.37) has been studied through in situ high-pressure powder X-ray diffraction. The ZIF-62 derivatives are observed to contract reversibly from an open pore (op) to a closed pore (cp) phase under hydrostatic mechanical pressure.
Importantly, the observed op-to-cp phase transition switches from the typical first order (discontinuous) to second order (continuous) with increasing the bim– fraction (to 17.5%). Rietveld refinements revealed that the second order transition is achieved by a continuous linker rotation. The mechanism that the void volume and the pore size of the material can be tuned continuously by adjusting the pressure was demonstrated.
To investigate the melting mechanism, a series of derivates of ZIF-4 (Zn(im)2) containing various amounts of cyano-functionalized imidazolate linkers was synthesized. The incorporation of electron-withdrawing cyano groups results in a drastic decrease in the melting temperatures. Density function theory (DFT) calculations revealed that the cyano groups weaken the dissociation of Zn–N bonds in the melting process. Remarkably, a particular liquid-liquid transition (LLT) of prototypical ZIF-4 remains in all cyano derivatives. The kinetic fragility of ZIF liquids has been demonstrated to be correlated with their micropore volume.
Overall, this work provides a guideline for controlling the mechanical responsiveness and melting behavior of MOFs by linker functionalization. The mechanically tunable MOFs open new possibilities for their application in pressure-switchable devices, membranes, and actuators. The porous glasses produced through controllable melting can further facilitate the manufacture of functionalized MOF glasses.
Einige Exemplare Metallorganischer Gerüstverbindungen (engl. Metal-Organic Frameworks, MOFs) zeigen eine beachtliche strukturelle Flexibilität als Reaktion auf externe Stimuli (z.B. Druck und Temperatur). Ihre responsives Verhalten kann dabei durch Substitution funktioneller Gruppen an der organischen Baueinheit (Linker) des Netzwerkrückgrates gesteuert werden. Kürzlich wurde berichtet, dass einige MOFs in der Lage sind, zu schmelzen und Gläser zu bilden und dass ihr Schmelzverhalten mit der Funktionalisierung der Linker in Zusammenhang steht. Darauf aufbauend wurden in dieser Arbeit die Mechanismen untersucht, welche die Responsivität und das Schmelzverhalten von MOFs infolge der Linkerfunktionalisierung (mit Benzo- und Cyanogruppen) steuern.
Das Hochdruckverhalten einer Reihe von Zeolithische Imidazolat-Gerüste (ZIFs) aus ZIF-62 (M(im)2-x(bim)x, M = Zn2+/Co2+, im– = imidazolat, bim– = benzimidazolat, 0.02 x 0.37) wurde durch in-situ-Hochdruck-Pulverröntgenbeugung untersucht. Es wurde beobachtet, dass sich die ZIF-62-Derivate unter hydrostatischem Druck reversibel von einer offenporigen (op) zu einer geschlossenporigen (cp) Phase umwandeln. Besonders ist hier, dass sich mit zunehmendem bim–-Anteil (auf 17,5%) der beobachtete Phasenübergang von op zu cp von erster Ordnung (diskontinuierlich) zu zweiter Ordnung (kontinuierlich) wechselt. Rietveld-Verfeinerungen zeigten, dass der Übergang zweiter Ordnung durch eine kontinuierliche Rotation Linker- Baueinheiten erreicht wird. Wie gezeigt, kann dadurch das Porenvolumen und die Porengröße des Materials durch Anpassung des Drucks kontinuierlich eingestellt werden.
Um ihren Schmelzmechanismus zu untersuchen, wurde eine Reihe von Derivaten von ZIF-4 (Zn(im)2) synthetisiert, die sich hinsichtlich ihres Inhalts an Cyano- funktionalisierten Imidazolat-Linkern unterscheiden. Durch den Einbau von elektronenziehenden Cyanogruppen kommt es zu einer drastischen Reduzierung der Schmelztemperaturen. Dichtefunktionaltheorie-Berechnungen (DFT) ergaben, dass dies daraus resultiert, dass die Cyanogruppen die Zn-N-Bindung schwächen und somit deren Dissoziation während des Schmelzvorgangs erleichtern. Bemerkenswerterweise bleibt der besondere Flüssig-Flüssig-Phasenübergang (LLT) des prototypischen ZIF-4
in allen Cyano-Derivaten erhalten. Außerdem ergibt sich eine Korrelation zwischen der kinetischen Zerbrechlichkeit von ZIF-Flüssigkeiten mit ihrem Mikroporenvolumen.
Insgesamt zeigt diese Arbeit einen Leitfaden für die Kontrolle des mechanischen Ansprechvermögen und des Schmelzverhaltens von MOFs durch Linkerfunktionalisierung. Solch mechanisch steuerbare MOFs eröffnen neue Möglichkeiten für ihre Anwendung in druckschaltbaren Geräten, Membranen und Aktuatoren. Außerdem schafft Kontrolle über ihr Schmelzverhalten Zugang zu weiteren, neuen funktionalisierten MOF-Gläsern.
Contents ... i
List of Abbreviations ... v
1 General Introduction ... 1
1.1 Metal-Organic Frameworks ... 1
1.1.1 Isoreticular Metal-Organic Frameworks ... 3
1.2 Zeolitic Imidazolate Frameworks ... 5
1.2.1 Beyond Zeolitic Topologies ... 6
2 Motivation and Aims ... 9
Part I Tunning the High-Pressure Response of ZIF-62 ... 13
3 Phase Change Materials (PCMs) ... 17
3.1 Phase Change MOFs ... 17
3.2 Responsive ZIFs ... 19
3.2.1 ZIF-4 ... 20
3.2.2 ZIF-8 ... 22
4 Tuning the Structure and Property of ZIF-62 by Linker Functionalization ... 25
4.1 Objectives ... 25
4.2 Single-Crystal X-ray Diffraction ... 27
4.3 Low-Temperature Powder X-ray Diffraction ... 28
4.4 High-Pressure Powder X-ray Diffraction ... 32
4.5 Reversibility of the Phase Transition ... 37
4.6 Compressibility, Bulk Modulus and Pressure-Volume Work ... 38
4.6.1 Compressibility () ... 39
4.6.2 Bulk Moduli (K) ... 40
4.6.3 Pressure-Volume Work ... 41
4.7 Structure Refinement and Analysis ... 43
4.7.1 Rietveld Refinements ... 44
4.7.2 Structure Discussion ... 47
4.7.3 Porosity Analysis ... 49
4.8 Conclusions ... 53
Part II Melting and Glass-Formation of Cyano-Functionalized ZIFs ... 55
5 MOF Liquids and Glasses ... 59
5.1 The Influence Factors of Melting... 59
5.2 Liquid-Liquid Transition (LLT) and Fragility ... 62
5.3 Mixed-Linker Functionalization of ZIF-4 ... 64
6 Melting and Glass Formation of Cyano-Functionalized ZIFs ... 67
6.1 Objectives ... 67
6.2 Crystalline ZIF Synthesis and Structural Characterization ... 68
6.3 Thermal Behavior, Melting and Glass Formation ... 71
6.3.1 Melting and Liquid-Liquid Transition (LLT) ... 71
6.3.2 Glass Formation of Cyano-Functionalized ZIF-4 ... 74
6.3.3 DFT Calculations of Model Structures ... 80
6.3.4 Attempts to Capture the Low-Density Amorphous (LDA) Phase ... 83
6.4 Porosity of the Crystalline and Glassy Phases ... 86
6.5 Kinetic Fragility of the ZIF Liquids ... 89
6.6 Conclusions ... 93
7 General Summary & Outlook... 95
8 Materials & Characterisations ... 105
8.1 Synthesis and Activation ...105
8.1.1 ZIF-4(Zn) and ZIF-62(M) ...105
8.1.2 Cyano-Functionalized ZIF-4 ...106
8.2 DFT Calculations ...109
8.3 Single Crystal X-ray Diffraction ...110
8.4 Powder X-ray Diffraction ...110
8.4.1 Laboratory Powder X-ray Diffraction ...110
8.4.2 High-Pressure Powder X-ray Diffraction ... 110
8.4.3 Variable-Temperature Powder X-ray Diffraction ... 112
8.5 Variable-Temperature X-ray Total Scattering ... 112
8.6 Thermal Analysis ... 113
8.6.1 DSC Upscans of Samples Preheated to Different Temperatures ... 114
8.6.2 Fragility Determination ... 114
8.6.3 Viscosity Calculation... 115
8.7 CO2 Sorption ... 115
8.8 Fourier-Transform Infrared Spectroscopy ... 116
8.8.1 For ZIF-62 Samples... 116
8.8.2 For Cyano-Functionalized ZIFs ... 116
8.9 1H Nuclear Magnetic Resonance (1H NMR) Spectroscopy ... 117
8.10 Microscopy ... 117
8.10.1 Optical Microscopy ... 117
8.10.2 Scanning Electron Microscopy ... 117
Bibliography ... 119
Appendix ... 135
Appendix to Part I ... 137
A.1 Infrared Spectroscopy ... 137
A.2 1H NMR Spectroscopy ... 137
A.2.1 1H NMR Analysis of Sample Homogeneity... 146
A.3 Single Crystal X-ray Diffraction ... 149
A.4 Low Temperature Powder X-ray Diffraction ... 153
A.5 Profile Refinements of VT-PXRD Patterns ... 155
A.6 Thermal Expansivity ... 160
A.7 High-pressure Powder X-ray Diffraction ... 165
A.8 Le Bail Refinements of HP-PXRD Patterns ... 173
A.8.1 ZIF-62(Zn)-bim0.02... 173
A.8.2 ZIF-62(Zn)-bim0.05... 176
A.8.3 ZIF-62(Zn)-bim0.17... 179
A.8.4 ZIF-62(Zn)-bim0.25 ...182
A.8.5 ZIF-62(Zn)-bim0.30 ...185
A.8.6 ZIF-62(Zn)-bim0.35 ...188
A.8.7 ZIF-62(Co)-bim0.27 ...190
A.8.8 ZIF-62(Co)-bim0.37 ...192
A.9 Compressibility ...194
Appendix to Part II ... 213
B.1 X-ray Diffraction ...213
B.1.1 Single Crystal X-ray Diffraction ...213
B.1.2 Powder X-ray Diffraction ...214
B.2 Infrared Spectroscopy ...226
B.3 1H NMR Spectroscopy ...229
B.4 Microscopy ...253
B.4.1 Optical Microscopy ...253
B.4.2 Scanning Electron Microscopy (SEM) ...258
B.5 Thermal Analysis ...262
B.5.1 Thermogravimetric Analysis and Differential Scanning Calorimetry ..262
B.5.2 Fragility Determination ...267
B.6 Variable Temperature X-ray Total Scattering...271
B.7 CO2 sorption...275
List of Publications ... 279
List of Abbreviations
∆EZn-N relative dissociation energies
∆Hcryst-LDL enthalpy of framework collapse
Ea,vis the activation energy
m fragility index
K bulk modulus
Tf fictive temperature
Tg glass transition temperature
Tcrystal-LDL transition temperature from crystalline phase to low
TLDL,peak peak temperature of transition to low density liquid
Tm melting temperature
Td decomposing temperature
Vpore micropore volume
4MR four-membered ring
5-Cl-2-mbim− 5-chloro-2-methyl-benzimidazolate 6-Cl-5-Fbim− 6-chloro-5-fluoro-benzimidazolate
6MR six-membered ring
ag amorphous glass
aT thermally amorphized
CN coordination network
cp closed pore
CP coordination polymer
CSD Cambridge Structural Database
DAC diamond anvil cell
DSC differential scanning calorimetry
FTIR spectroscopy Fourier-transform infrared spectroscopy
HDA high-density amorphous
HDL high-density liquid
HP-PXRD high-pressure powder X-ray diffraction
IUPAC International Union of Pure and Applied Chemistry IRMOF isoreticular metal-organic framework
LDA low-density amorphous
LDL low-density liquid
LLT liquid-liquid transition
MOF metal-organic framework
MQG melt-quenched glass
vii NMR spectroscopy nuclear magnetic resonance spectroscopy
np narrow pore
op open pore
PCM phase change material
PSD pore size distribution
PTM pressure transmitting medium
PXRD powder X-ray diffraction
RT room temperature
SAV solvent accessible volume
SBU secondary building unit
TGA thermogravimetric analysis
tpdc2− p,p′-terphenyl dicarboxylate
vdW van der Waals
XPDF X-ray pair distribution function
ZIF zeolitic imidazolate framework
1 General Introduction
1.1 Metal-Organic Frameworks
According to the hierarchical nomenclature from the International Union of Pure and Applied Chemistry (IUPAC), Metal-Organic frameworks (MOFs) are considered to be coordination networks (CNs) with organic ligands containing potential voids. The concept of MOFs was first introduced by Omar Yaghi in 1994 at the Material Research Society Meeting and has become more and more popular because of their porosity, flexibility and designability.[3–6] MOFs are conveniently constructed by modular chemical units, i.e., the inorganic building units ranging from mononuclear metal ions to complex metal-(oxo)-clusters, and the organic building units composed of multitopic ligands (also called linkers) typically containing oxygen or nitrogen donor groups (e.g., multidentate carboxylates, imidazolates, etc.). The inorganic building units are usually serving as nodes and the organic building units are usually linkers. The inorganic nodes are interconnected by organic linkers to form a porous coordination network (Figure 1.1). Thanks to the inorganic and organic syntheses, many different nodes and linkers are available for designing diverse MOFs.[7,8] Over the last two decades, several subfamilies of MOFs have been designed, such as Isoreticular Metal-Organic Frameworks (IRMOFs) and Zeolitic Imidazolate Frameworks (ZIFs). Other compounds, for example MIL-53 (MIL = Materials of Institute Lavoisier) [9–12], DUT-60 (Dresden University of Technology) [13–15], HKUST-1 (Hong-Kong University of Science and Technology) [16,17], NU-100 (Northwest University) [18–20] have also been synthesized. As of January 2020, a staggering number of 99 075 MOFs has been included in the MOF subset of the Cambridge Structural Database (CSD, 2020.0 release).
Figure 1.1: Scheme of a MOF constructed from inorganic nodes (metal ions, metal-oxo cluster, etc.) and organic linkers (multidentate carboxylates, imidazolates, etc.).
The design and synthesis of new MOFs are further instructed by the scope of reticular chemistry, which was proposed by O. Yaghi, M. O’Keeffe and their co-workers in 2003.[4,22] This conception depicts the chemistry of linking molecular building units by strong bonds to synthesize crystalline frameworks with open pores. It allows to obtain MOFs with particular topologies using specific nodes and/or linkers. The nodes are linked by the linkers on their coordinating sites. The geometry of the linker, especially its coordinating sites dictates the topology of the frameworks. In terms of their coordinating sites, the shape of the building units can be abstracted into so-called secondary building units (SBUs). The interpretation of SBUs of a series of building units is illustrated in Figure 1.2. With the help of SBUs, the network topologies can be easily identified and the frameworks with desired topologies can be freely designed by selecting suitable SBUs.
Metal-Organic Frameworks (MOFs) inorganic node
(Zn2+, Al3+, Cu2+, Co2+, etc.) metal-oxo cluster
e.g. carboxylates, imidazolates, pyrazole
3 Figure 1.2: Common secondary building units of inorganic nodes and organic linkers of MOFs. Reprinted with permission from Springer Nature, copyright 2003.
1.1.1 Isoreticular Metal-Organic Frameworks
The concept of iso-reticular chemistry facilitated the syntheses of MOF series possessing identical topology. A series of topologically identical MOFs has been achieved by utilizing the strategy that included isoreticulating metal ions and organic dicarboxylates.[12,14,18,24–26] This is particularly exemplified by MOF-5, one of the most investigated MOFs.[3,27,28] MOF-5 uses octahedral Zn4O(CO2)6 clusters as nodes, which are connected by the 1,4-benzenedicarboxylate (bdc2−) linkers. MOF-5 exhibits a primitive cubic (pcu) topology, showing a typical scaffold-like framework, whose representative structure can be viewed in Figure 1.3. Guest-free MOF-5 has a free volume of about 79.2% (calculated using the program cerius2, version 4.2), which gives it a low density of only about 0.59 g cm−3. Even though, MOF-5 is generally considered to be stable in terms of external stimuli, which does not change its volume
inorganic nodes SBUs organic linkers SBUs
over 4% upon removing/exchanging guest molecules, offering a suitable platform to further modify the structure.
Figure 1.3: The scheme of MOF-5 with the SBU of octahedral Zn4O(CO2)6 clusters and the bdc2− linker.
The prototypical MOF-5 is also called IRMOF-1, which has already been expanded to a series of isoreticular metal-organic frameworks (IRMOF-n, n is a chronological number) by linker functionalization. For example, IRMOF-2, IRMOF-3 and IRMOF-6 are respectively using bromo, amino and cyclobutyl substituted 1,4- benzenedicarboxylate (bdc2−) as linkers, IRMOF-8 is using a polycyclic aromatic hydrocarbon linker to prevent the interpenetration (i.e., the intergrowth of two or more frameworks in one structure without a chemical linking, which eliminates the porosity), and more substituting linkers are shown in Figure 1.4. Different linkers bring unique features to the frameworks,[30–32] thus the physical and chemical features
bdc2- Zn4O(CO2)6 MOF-5
5 of MOFs (e.g., pore volume, pore diameter, surface area, polarity) can be easily adjusted by linker functionalization.
Figure 1.4: Representation of IRMOF-n with possible linker substituents.
Based on the porosity and flexibility, combined with its designability, MOFs are promising in applications ranging from energy technologies of gas separation[33–35] and storage[36–43], particular fuel cells[38,40–44], and catalysis[45,46] to information technologies such as sensors[47–51], energy technologies[47,52–56][57,58], and even biotechnologies like molecular encapsulation or drug delivery[59–71]. Besides synthesizing new MOFs, the frontier of MOF studies now has been expanded to further functionalize the existing MOFs and try to break through previous high-technology applications.[4,55–58,60,72–77]
1.2 Zeolitic Imidazolate Frameworks
Zeolitic imidazolate frameworks (ZIFs) are an important subfamily of MOFs, which provides more than 250[78–83] out of nearly a hundred thousand MOF structures. ZIFs particularly adopt the imidazolate-type (Xim−) linkers to bridge the metal nodes of divalent cations M2+ (e.g., Mg2+, Mn2+, Fe2+, Co2+, Zn2+, Cd2+).[84–88] Each M2+ ion is tetrahedrally coordinated by four Xim− linkers to form an MN4 tetrahedron, which
IRMOF-1 (MOF-5) IRMOF-2
is the SBU of ZIFs. The SBUs are interconnected by the Xim− linkers to form a 3D network. The network can possess a variety of topologies, depending on the orientation of the SBUs. Every two SBUs connected through one Xim− linker forms a basic building block of ZIFs (Figure 1.5b). The bond angles of M-im-M (ca. 144°) and N- M-N (ca. 109.5°) in the ZIF building block are similar to that of Si-O-Si (ca. 140° - 160°) and O-Si-O (ca. 109.5°) in mineral silicates/zeolites (Figure 1.5a).[89–94] Due to this geometrical similarity, many ZIFs exhibit the topologies of zeolite minerals. The common topologies adopted from zeolites are sod (ZIF-8, ZIF-67, ZIF-7, ZIF-65, ZIF- 90), rho (ZIF-11, ZIF-12, ZIF-71) and gis (ZIF-6, ZIF-74, ZIF-75) as shown in Figure 1.7.[59,65,71]
Figure 1.5: Representative scheme showing the similarities of bond angles and building block geometry between zeolites/silicates (a) and ZIFs (b).
1.2.1 Beyond Zeolitic Topologies
However, the ZIFs are not linearly expanding as for the example of IRMOFs. ZIFs usually form an interweaved network rather than scaffold-like structures, because the M-N-M angles bridging ZIF building blocks are not straight. ZIF topology will change significantly if the imidazolate ring rotate around the M-N bonds. The orientation of the imidazolate ring is restricted by the steric effect from the neighboring groups. The steric effect of neighboring linkers can be modified by substituting functional groups on the imidazolate rings. Therefore, the orientation of imidazolate linkers can be arranged through the linker functionalization. In other words, the topology of ZIFs
Building blocks of silicates and zeolites
Building blocks of
zeolitic imidazolate frameworks (ZIFs)
O Si M
M–im–M angle ~ 144°
N–M–N angle ~ 109.5°
Si–O–Si angle ~ 140°- 160°
O–Si–O angle ~ 109.5°
7 can be conveniently manipulated by the linker functionalization, so that large structural diversity can be achieved.
Figure 1.6: Representation of the crystal structure of ZIF-4 (left) and the corresponding cag topology (middle). Unit cells are shown as thin black lines. The inorganic building unit of ZnN4 tetrahedron of ZIF-4 (right).
ZIF-4 is a prototypical ZIF using only the basic imidazolate (im–) as linkers, with the chemical composition M(im)2 (with M2+ = Zn2+[92,95], Co2+). The uninodal network feathers the cag topology (known from the mineral CaGa2O4, vertex symbol 220.127.116.11.6.6), where the metal nodes are tetrahedrally coordinated by the im– linkers to form the inorganic building unit of the MN4 tetrahedron (Figure 1.6). The simple construction principle of ZIF-4 (using only single metal ions and the basic im– linkers) allow more predominance of responsive phase behavior. ZIF-4 exhibits the reversible transitioning from an open pore (op) form to a closed pore (cp) form either upon mechanical compression[98,99] or by cooling the material to cryogenic temperatures. ZIF-4 is also the first MOF to be demonstrated to melt and form a glass after vitrification, upon heating before decomposition.[100,101]
As expected, more and more topologies, which were not observed in natural zeolites have been realized in ZIFs, through adopting functionalized imidazolate linkers. The novel topologies include the important cag topology (obeyed by ZIF-4, ZIF-62, TIF-4)[92,96], which validates the particular phase transition[97,98,102] and the unique
inorganic building unit
thermal behavior[100,103]. The other topologies including their representative ZIF structures (e.g., zni (ZIF-zni, ZIF-61, etc.)[94,104] and moz (ZIF-100)) are shown in Figure 1.7. Worth to mention that the substituents will not only change the steric bulk, but also affect the mechanical property and thermal behavior of the framework.
Figure 1.7: Representative ZIFs containing porous spaces (in yellow) are catalogued by their topologies (showing in schemes of nets and tiles, indicated by three-letter symbols).[78,89] Reprinted with permission from AAAS and ACS publications.
2 Motivation and Aims
Up to now, nearly hundreds of thousands of MOF structures have been synthesized based on the modular construction principle. As a class of new materials, MOFs are well-known for their porosity, flexibility and designability. These properties render MOFs potential candidates for applications in various fields, such as gas storage, separations, chemical sensing, controlled drug release or as shock absorbers.
MOFs’ designability is owing to the structural diversity of inorganic and organic building units. To design new MOFs, one way is diversifying the organic linkers by implementing functional groups. For example, a series of ZIF-62 has been derived from the prototypical ZIF-4 with incorporating various amounts of benzimidazolate functionalization. The balance of enthalpy and entropy in the framework will be affected through functionalizing the organic linkers, which will influence the flexibility of the MOFs.
Flexible MOFs exhibit responsive phase behaviors under external stimuli (e.g., pressures and temperatures). Previous results have shown that ZIF-4 undergoes a phase transition from an open pore (op) to a closed pore (cp) phase in response to the stimuli of pressure and temperature. The op-to-cp phase transition of ZIF-4 is first order and showing an abrupt jump in the volume change, which makes it challenging to fine-tune the related properties. Besides that, due to the strong M-im-M bonds and consequently high thermal stability, ZIF-4 was recently reported to be able to melt and form glasses before decomposition. However, the material first recrystallizes to a denser ZIF-zni (ZIF structure with zni topology) phase and the subsequential melting temperature is too high and close to the decomposition temperature, which is not beneficial for the glass manufacture.
Functionalizing the linkers in the framework offers the advantage to tune the responsive behaviors of MOFs. However, the mechanism to precisely control MOFs’
responsive behaviors by linker functionalization is yet to be established.
As featuring the single metal node (Zn2+ or Co2+) and basic imidazolate (im−) linkers, ZIF-4 is adopted as the platform for further functionalization in this work.
Part I – Mechanically Responsive ZIF-62
ZIF-4 initially shows the first order op-to-cp phase transition. In order to enhance the framework from pore collapse, bulky benzimidazolate (bim−) linker are incorporated as secondary linkers. ZIF-62 [M(im)2–x(bim)x] is a series of derivates of ZIF-4 with a certain concentration of bim− substituents. The phase behavior of ZIF-62 will be in situ monitored upon pressurizing or under cryogenic conditions through powder X-ray diffraction with synchrotron radiation. Considering the steric effect from the bim− substituents, the following question has to be addressed: How will the op-to-cp phase transition and associated properties be modified by the concentration of bim− linkers?
Part II – Cyano-functionalized ZIF-4 Glasses
The cyano groups exhibit an electron-withdrawing effect from the attached moieties, which can delocalize the charges and weaken the associated bonds. Through functionalizing with either 4-cyanoimidazolate (CNim−) or 4,5-dicyanoimidazolate (dCNim−), a series of ZIF-4-CNx/dCNx samples will be synthesized. The melting temperatures of ZIF-4 are expected to be much lower, due to the weakening of Zn-N bonds. Prototypical ZIF-4 exhibits the particular liquid-liquid transition (LLT), which shows an exothermic framework collapse to a low density liquid phase and a subsequent transition to a high density liquid phase. The LLT is of great interesting to understand the physicochemical parameters and the thermodynamics of the framework collapse. However, this LLT disappears for the benzannulated ZIFs with a small amount of bim− functionalization (e.g., x 0.05 for ZIF-62(Zn)-bimx). The size of cyano groups is not as bulky as bim− and they are exhibiting the electron- withdrawing effect. These attributes naturally raise up the curiosity, how the melting behavior of ZIF-4 will be modulated by the cyano functionalization?
11 In the following chapters, tuning the responsive phase transition of ZIF-62 and modulating the melting behavior of cyano-functionalized ZIF-4 by linker functionalization of bim− or CNim−/dCNim− will be investigated and presented in Part I and Part II, respectively.
Tunning the High-Pressure
Response of ZIF-62
The work presented in this part has been published in the following peer-reviewed research article. This publication (text and figures) is subsequently reprinted or adapted with the permission of the publisher. Author contributions are distinguished below.
J. Song, R. Pallach, L. Frentzel-Beyme, P. Kolodzeiski, G. Kieslich, P. Vervoorts, C.
L. Hobday, S. Henke, Angew. Chem. Int. Ed. 2022, 61, e202117565.
J.S. synthesized the ZIFs and collected and analyzed PXRD, SCXRD, IR spectroscopy and NMR spectroscopy data. J.S. performed the crystallographic analysis. R.P. and S.H. helped with the Rietveld refinements. L.F.-B. helped with the initial syntheses.
J.S., R.P., L.F.-B. and P.K. performed HP-PXRD with G.K., P.V. and C.L.H.
performing preliminary experiments. R.P., L.F.-B. and S.H. performed the VT-PXRD experiments. J.S. and S.H. wrote the paper. All authors participated in discussing the data and contributed to revising the manuscript.
The high-pressure behavior of flexible zeolitic imidazolate frameworks (ZIFs) of the ZIF-62 family with the chemical composition M(im)2-x(bim)x is presented (M2+ = Zn2+, Co2+; im– = imidazolate; bim– = benzimidazolate, 0.02 ≤ x ≤ 0.37). High-pressure powder X-ray diffraction shows that the materials reversibly contract from an open pore (op) to a closed pore (cp) phase under a hydrostatic pressure of up to 4000 bar.
Sequentially increasing the bim– fraction (x) reinforces the framework, leading to an increased threshold pressure for the op-to-cp phase transition, while the total volume contraction across the transition decreases. Most importantly, the typical discontinuous op-to-cp transition (first order) changes to an unusual continuous transition (second order) for x ≥ 0.35. This allows finetuning the void volume and the pore size of the material continuously by adjusting the pressure, opening new possibilities for MOF-based pressure-switchable devices, membranes, and actuators.
3 4 5 6 7
0 1000 2000 3000 4000
Pore diameter / Å
Pressure / bar
0.01 0.03 0.05 0.07 0.09 0.11 Differential pore volume / cm3 g-1 Å-1
3 Phase Change Materials (PCMs)
Phase transitions in solid materials are of fundamental importance for a number of applications across engineering, chemistry, physics and data storage.[106–111] Phase change materials (PCMs) can switch reversibly between different phases with distinct physical properties (e.g., an amorphous and one or more crystalline phases) depending on their environments. A better understanding of the structural responses to the environmental stimuli is of paramount importance to understanding the responsive mechanism of PCMs. These responsive materials, which drastically change their chemical or physical properties under external stimuli, are significant for developing novel energy-efficient technologies.[7–9]
3.1 Phase Change MOFs
Due to the combination of the relatively weak ligand-to-metal coordination bonds (at least compared to the strong covalent bonding) and various modes of stabilizing dispersion and dipolar interactions between the organic building units, a number of MOFs show flexibilities through reversible first order phase transitions between two distinct states of essentially different porosity and density in response to various stimuli.[30,112–114] The most prominent stimuli are the ad-/desorption of guest molecules or changes in temperature.[76,112,115–118] One of the best studied examples is the extreme transition of the carboxylate-based MOF MIL-53 (MIL = Materials of Institute Lavoisier, M(OH)(bdc); M3+ = Al3+, Cr3+, Fe3+, Ga3+; bdc2– = 1,4-benzenedicarboxylate).[12,119,120] MIL-53 (with M3+ = Al3+, Cr3+) features an expanded large pore (lp) form when guest-free and at room temperature.
Adsorption of water causes a drastic contraction to a narrow pore (np) form featuring only about 40% of the unit cell volume of the original lp form (Figure 3.1). This
phase transition of MIL-53 was coined ‘breathing’ and can also be triggered by cooling to cryogenic temperatures. A large body of previous work also demonstrated that the responsive properties of flexible MOFs could be adjusted by exchanging or tuning the corresponding inorganic or organic building units of the materials.[76,115,116,118,122]
For example, the alkoxy functionalized DMOFs exhibit the negative thermal expansion. By exchanging metal ions or functionalizing the organic linker, the materials’ responsiveness can be adjusted for a particular application (e.g., micro sensors or switches).[24,31,76,115,116,123] Such remarkable structural flexibility and adjustability opens the door for new and functional properties, which can be exploited in applications ranging from gas capture[36,37] and separation[33,34] to fuel cells, supercapacitors and catalysis[45,46].
Figure 3.1: Wine-rack structure of MIL-53(Al) showing the transition between large pore (lp, left side) and narrow pore (np, right side) through ad-/desorption of water at ambient temperature and pressure. Gray octahedra: AlO4(OH)2; black spheres: carbon; grey spheres:
oxygen. Figure from reference  with permission from John Wiley and Sons.
Besides their response to gas sorption and temperature, the reaction of flexible MOFs to mechanical pressure received more and more attention recently, not only due to its relevance for shaping and pelletizing MOFs for applications in catalysis and sorption, but also for the exploration of new applications, such as shock absorbers or dampers.[98,124–128] Several derivatives of the MIL-47/MIL-53 family (M(X)(bdc); M = V4+, Cr3+, Al3+; X = O2–, OH–, F–; bdc2– = 1,4-benzenedicarboxylate) have been demonstrated to undergo a first order phase transition from a large pore (lp) to a narrow pore (np) phase under mechanical pressure.[124,125,127,129] Due to the wine-rack-
19 like structure of these materials, the lp-to-np transition is highly anisotropic, involving a strong framework compression in one direction, which is geometrically coupled to an expansion in the perpendicular direction. A strongly related structural behavior has also been demonstrated in pillared-layered MOFs of the type M2(fu-bdc)2(dabco) (M = Zn2+, Cu2+; fu-bdc2– = dialkoxy-functionalized bdc2–, dabco = 1,4-diazabicyclo[2.2.2]octane), which possesses a similar wine-rack-like structure.[25,115,130–132] For MIL-47/MIL-53 materials as well as the pillared-layered MOFs, it was shown that the nature of the metal ion as well as the functionalization of the organic linker, influences the responsive transition of the lp-to-np transition significantly.[125,127,129,131,133,134]
3.2 Responsive ZIFs
ZIFs (i.e., imidazolate-based MOFs with divalent metal ions) originally possess a single metal node and basic imidazolate (im–) linkers. The metal nodes are usually interconnected through the im– linkers with obeying certain topologies. The functionalization of ZIFs is mainly focusing on substituting the im– rings. For example, ZIF-7 (Zn(bim)2) was synthesized with benzimidazolate (bim–) functionalization and featuring a sod topology. ZIF-7 shows intriguing phase behaviors through interacting with various guest molecules. ZIF-7 will already contract to a narrow pore (np) phase after activating from the solvent of N,N-dimethylformamide (DMF) molecules. The large pore (lp) phase of ZIF-7 can be recovered from the np phase via re-adsorption of guest molecules of N2, CO2 and other gaseous hydrocarbons[137–141]. It is noteworthy that the threshold pressures required for the gate-opening of ZIF-7 depend heavily on the guest-host molecular interactions.
Compared to the well-studied responsive behavior of a large number of carboxylate- based MOFs[11,15,17,19,20,43–48], the pressure-responsive behavior of ZIFs is so far less explored. The vast majority of studies on the mechanical behaviors of ZIFs concentrate only on a few critical ZIF structure types, e.g., ZIF-4 and ZIF-8 (Figure 3.2).
Figure 3.2: Representation of crystal structures (on the left) with corresponding solvent accessible volumes (SAVs, shown in dark yellow, on the right side) of ZIF-4 (CSD CODE:
VEJYUF) and ZIF-8 (CSD CODE: VELVOY). Color code: zinc, green; nitrogen, blue;
carbon, grey. H atoms and solvent molecules are not shown for clarity. The SAVs have been calculated with the Mercury software using a probe radius of 1.5 Å and a grid spacing of 0.2 Å.
ZIF-4 (M(im)2, M = Zn2+/Co2+) is a crystalline porous material with possessing the cag network topology[78,92,95,96] (introduced in Section 1.2.1) and crystallizing in the orthorhombic space group Pbca. Guest-free ZIF-4 has a density of 1.22 cm3/g and features an interconnected network of pores with solvent accessible volume (SAV) of about 25.9% (see in Figure 3.2). In terms of the complexity of the phase behavior, ZIF-4 is likely one of the most exciting ZIFs studied thus far.
Desolvated ZIF-4(Zn) was first reported to transform from its conventional open pore (op) phase to a drastically contracted closed pore (cp) structure when cooled to temperatures below 140 K under vacuum. ZIF-4(Zn) retains the cag topology and space group symmetry (Pbca) but isotropically contracts almost by about 23%, which
SAV = 25.9%
SAV = 49.6%
21 is achieved by substantial rotations of the im– linkers (up to 69.3°, C3n ring in Figure 3.3b) about the Zn–N bonds. The concerted rotation of the im– linkers results in a 3D inward folding of the framework, leading to a drastic reduction of the void fraction of 77%.
Figure 3.3: (a) Reversible op-to-cp phase transition of guest-free ZIF-4(Zn) under external stimuli. Zn, N and C atoms are shown in yellow, blue, and grey. The void surface is shown in green. (b) Overlay of a fraction of the op (in dark color) and cp (in pale color) crystal structures of ZIF-4 prepared by selecting one crystallographically independent im– linker as a point of reference.Figure adapted from citations  (© 2015 WILEY-VCH Verlag GmbH
& Co. KGaA, Weinheim) and  (with permission from the Royal Society of Chemistry).
Desolvated ZIF-4(Zn) as well as ZIF-4(Co) were later revealed to undergo a similar op-to-cp phase transition under mechanical compression by in situ high-pressure powder X-ray diffraction (HP-PXRD) experiments with synchrotron radiation.
ZIF-4(Zn) requires a threshold pressure of ca. 280 bar to initiate the phase transition, while ZIF-4(Co) needs about 500 bar. ZIF-4(Zn) shows a volume reduction of 21% and ZIF-4(Co) shows a contraction of 19%. But the found cp phase features additional Bragg reflections compared to the established low temperature cp phase, which suggests a reduction in symmetry owing to pressurization. The reversibility depends on the metal cations: ZIF-4(Zn) requires subsequent heating to transfer back to the op phase, whereas ZIF-4(Co) immediately returns to the op phase after decompression.
For the experiment above, a non-penetrating pressure transmitting medium (PTM) of Fluorinert FC-70 was used. It’s worth to mention that the influence of using different PTMs led to very different conclusions of the pressure induced behavior, e.g., amorphization. The measurement using small molecule PTM (volume ration of
methanol : ethanol = 4 : 1) shows a much higher amorphization pressure (1.49 – 4.54 GPa). The smaller PTF molecules will penetrate into the frameworks and the interaction between guest-host molecules enhanced the framework from getting amorphized. In addition, the measurement using Daphne Oil 7474 as a PTF did not show the cp phase, which may be attributed to 100 times faster pressurizing rate.
As mentioned at the beginning of Section 3.1, the op-to-cp phase transition is actually governed by the delicate balance between enthalpy (e.g., dispersion interaction and polarization) and entropy (e.g., vibrational or configurational degrees) to the free energy landscape, which can be affected by external stimuli (e.g., pressure and temperature).[114,118,144–146] The thermodynamic driving force of the op-to-cp phase transition is the higher enthalpic stability of the cp phase, which arises from attractive dispersion interactions between the molecular building units. The dispersion interaction between the organic linkers is the key factor to stabilize the cp phases.[147,148] Once the external stimuli are applied (compression or contraction), the linkers move closer to each other and the dispersion interactions become stronger.
Thus, the cp phase is enthalpically more favorable under pressurizing or cooling. At higher temperatures or lower pressures, the op phase is stabilized by vibrational entropy.[149,150] It is expected that the dispersion interaction will also be affected by the implementation of functional groups at the organic building unit of the framework, owing to the addition on dispersion interactions between the functional groups and the framework backbone.[25,151,152]
ZIF-8 [Zn(mim)2], composed of divalent zinc cations and 2-methyl-imidazolate (mim−) linkers, is one of the most extensively investigated ZIFs, and it has also been already commercialized because of its exceptionally thermal and chemical stability and high porosity[57,68]. ZIF-8 retains the archetypal sodalite (sod) topology (vertex symbol: 18.104.22.168.6.6.) and features one type of cage with a diameter of ca. 12.5 Å (Figure 3.2). The open sodalite pores are described by six-membered rings (6MRs) and four-membered rings (4MRs), resulting in a structure with about 50% SAV.
23 ZIF-8 was previously considered to be relatively rigid due to pressurizing with the penetrating PTFs.[77,142,155] The experiment was conducted on a single crystal of ZIF-8 using a mixture of methanol/ethanol as a PTM in a diamond anvil cell (DAC).
ZIF-8 requires a relatively high threshold (about 1.47 GPa) to undergo the transition from the ambient phase (AP) (Figure 3.4a) to a high pressure phase (HP) (Figure 3.4b). The structure of the HP phase though remains the space group of the AP phase. The phase transition involves the rotation of the mim− linkers around the Zn-mim-Zn axis, where the angle between the planes of the mim− rings and the crystallographic planes along the a axis (100 plane) increased from an acute angle (ca.
30°) to a right angle (Figure 3.4). Interestingly, the pore aperture increased while the re-orientation of the mim− groups, i.e., the effective window size of the 6MRs increased from ca. 3.0 Å to ca. 3.6 and the 4MRs from ca. 0.8 Å to ca. 2.2 Å, which is because the methanol/ethanol molecules penetrated into the frameworks and interacted with the linkers. The unit cell volume also expends from 4901 Å3 (ambient pressure) to 4975 Å3 (1.47 GPa). However, ZIF-8 is known to be indeed soft later, for example it exhibits an extremely low shear modulus.
Figure 3.4: Pressure induced phase transition (threshold at 1.47 GPa) from (a) ambient- pressure (AP) to (b) high-pressure (HP) phases of ZIF-8, noticeable by mim− linker reorientation. Gray tetrahedra: ZnN4; black spheres: carbon or nitrogen atoms; hydrogen atoms were omitted for clarity. Figure from , Copyright © 2009 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim.
4 Tuning the Structure and Property of ZIF-62 by Linker Functionalization
There are two fundamental types of phase transitions of materials, first order or second order. The first order phase transition is discontinuous concerning the change of volume (the first derivative of free energy), while the second order phase transition is continuous on the volume change but discontinuous with respect to the second derivative of free energy (e.g., heat capacity and compressibility). This defines that the first order phase transition is indicative through abrupt changes in the unit cell volume (Figure 4.1a), and the phase transition switches into second order when the discontinuities only appear in the slope of the volume change (Figure 4.1b).
Figure 4.1: Representative illustration of volume changes of first order (a) and second order (b) phase transitions with applying pressures. pc indicates the critical pressure of the phase transition.
First order transition Second order transition
The op-to-cp phase transition of ZIF-4 is typically first order showing an abrupt jump in the volume change, which makes it challenging to tune the phase transition related porosity. As indicated above, the linker functionalization has influence on the responsive behaviors. However, the precise influence of such functionalization on the responsive phase behavior is hard to predict. In order to fine-tune the phase transition, a methodology that targets the tuning of the supramolecular mechanics of responsive MOFs must be developed.
Figure 4.2: (a) Scheme of the building blocks of ZIF-62. (b) Single crystal structure of guest-free ZIF-62 (op phase) from this work showing the unit cell (left) and the asymmetric unit (right) with the partially occupied bim– linkers at the crystallographically independent positions 1 and 2 highlighted.
The work in this part will thoroughly demonstrate that the high-pressure mechanical behavior of a flexible MOF system can be very precisely adjusted by applying the concept of mixed-linker functionalization. ZIF-4 was adopted as a flexible MOF platform to be further functionalized. It is well established that parts of the im–
M2+= Zn2+, Co2+
27 linkers in ZIF-4 can be exchanged for bulkier benzimidazolate (bim–) linkers while network structure and topology remain unchanged. The corresponding materials of the general chemical formula M(im)2–x(bim)x are known under the name ZIF-62 (Figure 4.2) and have first been reported for M2+ = Zn2+ and x = 0.25. The cobalt derivative with x = 0.30 was described later. It has been recently demonstrated that ZIF-62 and ZIF-4 form a continuous solid solution with x ranging from 0 (for ZIF-4) to 0.35.
In the following chapters of this part, the structural behavior of a series of eight different solid solutions of the ZIF-62 family (denoted as ZIF-62(M)-bimx, M = Zn2+
or Co2+ and 0.02 x 0.37) with high-pressure (HP) powder X-ray diffraction (PXRD) in the pressure range from ambient pressure up to 4000 bar will be investigated.
Supporting insights in the corresponding low temperature behavior of the materials are obtained with variable temperature (VT) PXRD in the range from 300 K down to 100 K. It is demonstrated that the HP phase behavior of the materials can be systematically tuned by precisely adjusting the fraction (x) of bim– in the material, leading to (i) a reinforcement of the frameworks and a shift of the op-to-cp transition pressure to higher pressures, (ii) a concomitant reduction of the volume change (∆V) across the transition and (iii) the evolution from a discontinuous (first order) to a continuous (second order) phase transition with increasing x. Structure refinements based on the HP-PXRD data (Rietveld method[163,164]) elucidate that the continuous change from the op-to-cp phase allows adjusting the pore volume and pore size of the material precisely by selecting the corresponding pressure. The work here will provide a guideline for the targeted finetuning of the supramolecular mechanics of flexible MOFs, setting the stage for their application in pressure-switchable membranes, nanodampers or nanoscopic pressure actuators.
4.2 Single-Crystal X-ray Diffraction
Guest-free single crystals of all ZIF-62(M)-bimx solid solutions were studied with single crystal X-ray diffraction (see Figure 4.2b and Section A.3 of Appendix for the crystallographic tables). All compounds possess the orthorhombic space group Pbca
and form the cag topology, featuring two independent M2+ cations and four independent imidazolate-type linkers in the asymmetric unit. In all compounds, the bim– linkers are partially occupying two out of the four crystallographically independent linker positions (highlighted as position 1 and 2 in the asymmetric unit in Figure 4.2b). For x = 0.02, bim– could only be located at position 1, while bim– partially occupies both positions 1 and 2 for x ≥ 0.05. The occupancies of bim– at the two crystallographically independent positions are compiled in Table 4.1. It is noteworthy that the bim– linker at position 2 features a significantly different orientation than the smaller im– linker at the same position, so the unfavorable steric interactions with neighboring linkers are avoided.
Table 4.1: Occupancies of bim– on the two crystallographically independent positions im1 and im2 determined by single crystal diffraction.
Position ZIF-62(Zn)-bimx ZIF-62(Co)-bimx
0.02 0.05 0.17 0.25 0.30 0.35 0.27 0.37 1 0.04
(fixed) 0.104(2) 0.173(2) 0.396(3) 0.355(2) 0.120(2) 0.361(3)
2 - 0.05
(fixed) 0.236(2) 0.327(2) 0.204(3) 0.345(2) 0.420(2) 0.379(3)
4.3 Low-Temperature Powder X-ray Diffraction
The low temperature behavior of selected representatives of the ZIF-62(M)-bimx materials was compared to the behavior of the highly flexible parent compound ZIF-4(Zn). High-resolution VT-PXRD patterns of carefully ground samples were recorded at beamline P02.1 of PETRA III at DESY (Deutsches Elektronen Synchrotron, Hamburg, Germany) upon cooling the materials from 300 K down to 100 K with data collected every 10 K (see in Section A.4 of Appendix). In accordance with a previous report, the op-to-cp transition of ZIF-4(Zn) starts at 190 K and is completed at 110 K. Except for ZIF-62(Zn)-bim0.02, all of the studied solid solutions ZIF-62(Zn)-bimx remain in the op phase when cooled to 100 K (Figure 4.3 right and
29 Section A.4 of Appendix). ZIF-62(Zn)-bim0.02 shows weak reflections associated to the cp phase appearing in the VT-PXRD patterns at temperatures below 150 K (Figure 4.3 left). However, the cp phase remains a minority in the diffraction pattern even at 100 K. These results signify that already tiny amounts of bim– have a decisive influence on the potential energy landscape of these materials and thus hamper the transformation to the enthalpically favored cp phase. Note that for x = 0.02, only 1%
of all linkers in the material are bim– (equal to only 0.32 bim– linkers per unit cell), while the others are the smaller im– linkers.
Figure 4.3: Stacked VT-PXRD patterns for ZIF-4(Zn) at the left and ZIF-62(Zn)-bim0.35
at the right collected during cooling down from 300 K to 100 K with 10 K per step and a subsequent return to 300 K.
Based on profile fits (Le Bail method, see in Section A.5 of Appendix), the coefficients of thermal expansion (CTE) for the op phases of the ZIF-62(M)-bimx
materials were derived from the temperature-dependent PXRD data. The thermal expansivity () as a function of temperature has been determined along each crystallographic axis in the range from 100 to 300 K (140 to 300 K for ZIF-4 and 110 to 300 K for ZIF-62(Zn)-bim0.02). The refined lattice parameters and the unit cell volume were fitted using an nth order polynomial function (1) or an exponential function (2) as suitable: